# dielectric properties of dipolar .dielectric properties of dipolar solids 401 for paraffins both

Post on 04-Jun-2018

214 views

Embed Size (px)

TRANSCRIPT

By H. F r o h l ic h , H. H. Wills Physical Laboratory, University of Bristol

{Communicated by N. F. Mott, F.R.S.Received 1 February 1945)

A. quantitative theory of the dielectric properties of crystalline solids consisting of dipolar long-chain molecules is developed (one dipole per molecule). In these solids the dipoles are concentrated in dipolar planes. In the ground state the dipolar planes have a permanent polarization, but usually the polarizations of successive planes have opposite directions. The static dielectric constant rises with increasing temperature up to a critical temperature T 0 and then decreases. At T0 the substance has a phase transition of the second kind. Comparison with experiments by Muller on a solid ketone lead to good agreement.

For chains with an even number of C-atoms metastable states with a permanent polarization are predicted, and a method to reach these states is discussed.

The interaction between dipoles plays a predominant role at temperatures below T0. It is shown that Lorentzs or Onsagers methods are invalid in this temperature range.

1. I n t r o d u c t io n

Dipolar solids consisting of long-chain molecules find a wide application as dielectrics. The most im portant of them, e.g. plastics, have a fairly complicated structure. One can hardly hope to reach a full understanding of their dielectric properties unless the dielectric behaviour of long-chain solids with a simple structure (e.g. solid ketones) is understood first. We shall, therefore, in the present paper develop a quantitative theory of the dielectric properties of simple crystalline solids consisting of long-chain molecules.

Substances of this type have already been investigated in a previous paper (Frohlich & Sack 1944, quoted as I), where it was shown that the methods usually used to account for the interaction between dipoles become invalid below a temperature T0 where 1cT0 is of the order of the dipolar interaction energy. Since T0 may be fairly high (for ketones it approximately coincides with the melting-point), a new method must be found to treat dipolar interaction. As was shown in I the dipoles undergo an order-disorder transition near the temperature T0. Approximate methods have been developed to deal with these transitions, and it will be seen tha t they can be used in the case of the substances discussed here.

As a main result it will be found that the static dielectric constant increases with temperature up to T0 and then decreases ( 3). Experiments by A. Muller (1938) on solid ketones lead to good agreement with the present results, as will be shown in 4. Moreover, from a discussion of structure (2), a number of interesting conclusions concerning the possible existence of a permanent polarization can be drawn. Experiments to check these conclusions will be suggested in 4.

I t will be of interest to notice that as in I the internal field acting on a dipole is not proportional to the macroscopic polarization. Thus an application of the method of the Lorentz field would lead to wrong results for the substances discussed in this paper.

* Based on report L/T 147 of tbe British Electrical and Allied Industries Research Association (E.R.A.).

D ielectric properties o f dipolar solids *

r 3 9 9 1

on July 5, 2018http://rspa.royalsocietypublishing.org/Downloaded from

http://rspa.royalsocietypublishing.org/

400 H. Frohlich

2. S t r u c t u r e a n d p r o p e r t ie s o f t h e g r o u n d st a t e Throughout this paper discussion will be restricted to crystalline solids consisting

of long-chain molecules each of which contains one dipole. In solids such molecules form plane zigzags, and it will be assumed th a t the dipole lies in the chain plane and is perpendicular to the chain axis, as is probably the case for ketones. In the simplest case these solids have a paraffin structure, i.e. according to Muller (1928) the molecular chains are arranged in layers whose thickness is approximately equal to the chain length. W ithin such a layer the molecules form rectangular cells with side length a, 6, c, where a ~ 5 A, 6 ~ 7*5 A and c slightly larger than the chain length. As discussed in I, each molecule has two equilibrium positions with opposite dipole direction. In the ground state the paraffin structure requires th a t they are oriented in such a way th a t they are nearly parallel as shown in figure 1. I t will be shown below th a t this also corresponds to the lowest interaction energy between the dipoles of one layer.

F igure 1. Dipolar structure of the ground state.

In such a structure all the dipoles of one layer lie in one plane (perpendicular to the chain axis) which will be Called the dipolar plane. The unit cell of the dipoles of a dipolar plane is shown in figure 1. In the ground state these dipolar planes are thus polarized in the 6-direction, and it is of great importance for the behaviour of the whole crystal to know the relative direction of the polarization of successive dipolar planes. First, then, consider tne position of successive layers in paraffins. According to Muller (1929) distinction m ust be made between two cases, according to whether the number of C-atoms of a chain is even or odd. Figure 2 shows the positions of two successive layers for the two cases. Now attach a dipole to each molecule a t distances cx and c2 from the two ends, i.e. + c2 = chain length. For both even and odd chains there exist now two possibilities. Except for the gap between the chains the distance between successive planes is (a) cx + c2, or (6) it is alternately 2cx and 2ca. Figure 3 shows th a t for odd chains both cases lead to opposite directions of the polarizations of successive dipolar planes. For even chains, however, this is only so in case (6), whereas in case (a) successive- layers have the same direction of polarization. This latter case will thus lead to a strong polarization of the crystal with all dipoles nearly parallel, while in the other cases the polarizations of successive layers cancel.

on July 5, 2018http://rspa.royalsocietypublishing.org/Downloaded from

http://rspa.royalsocietypublishing.org/

401Dielectric properties of dipolar solidsFor paraffins both oases (a) and ( b)are identical. Their energies, therefore, differ

only in the contributions of the dipoles. To calculate the dipolar interaction energy notice tha t the distance between neighbouring dipoles within a dipolar plane is less than 5 A, and is thus much smaller than the distance between neighbouring planes (unless the chain length is very small). First, then, one may calculate the interaction energy of a dipole with all the dipoles of the same dipolar plane, and then consider its interaction with the other dipolar planes. As in I, we assume the dipoles to be dispersed in a continuous medium with dielectric constant e^. The interaction energy between two dipoles whose distance is r is then given by

odd evenFiotJBE 2. Position of paraffin

chains in the ground state.

odd evenF igure 3. The two possible positions of

dipoles in the ground state.

where and p2 are the dipole moments of the two dipoles respectively. According to figure 1 the dipoles form an angle of about + 30 with the b axis. Thus their components fia and fib in the a-b frame are given by

Ha = /isin ( 30) = | , = cos ( 30) = (2)|

The interaction of the central dipole of figure 1 with its four nearest neighbours is thus given by (considering that b/a = 1-5)

V | 7 1 , 9\ 3 / .e ^ L l 4 4/ 3*25\ 2 2

3-3ft**

To this interaction the contributions of the further distant dipoles of the same dipolar plane have to be added. This, however, is very small. Taking a total of twenty neighbours the interaction energy becomes

w ___- a2 + b2

Vol. 185. A. 36

on July 5, 2018http://rspa.royalsocietypublishing.org/Downloaded from

http://rspa.royalsocietypublishing.org/

402 H. FrohlichI t is thus seen tha t the main contribution is due to the interaction between nearest neighbours. This is of great importance for the calculation of the interaction in the excited states ( 3). I t is due to the strongly anisotropic structure of long-chain substances. In other crystals the nearest neighbours frequently contribute only a small fraction to the total dipolar interaction energy.

Since according to I each dipole has two equilibrium positions with opposite dipole direction, other structures can be considered in which some of the arrows in the unit cell in figure 1 have the opposite direction, and which would lead to a vanishing polarization of a dipolar plane. I t is found th a t they all lead to a higher interaction energy between dipoles than the arrangement of figure 1.

To obtain the total interaction of a dipole with all other dipoles, its interaction with the other dipolar planes must be added. In view of their large distance it seems reasonable to consider a dipolar plane as a two-dimensional continuum with a constant polarization in the 6-direction (dipole moment aJ3ju,J2 per surface ab/2). This would lead to a reduction of the interaction between a dipole and a dipolar plane to an interaction of the dipole with the charge a t the circumference of the dipolar plane. This latter interaction energy vanishes if the dipolar plane becomes infinitely large. In order to check this result, Mr R. Sack kindly calculated th a t the interaction energy between a dipole and an infinite dipolar plane a t a distance z is of the order of magnitude

I87T*jpe~Z7rzlb,

which is thus about eZnzlb/100 times smaller than the interaction between neighbouring dipoles. For a distance of z~ 20 A (30 A) this leads to a factor 1010 (1014). I t thus seems to be a very good approximation